identificaci³n de arcillas
Post on 28-Apr-2017
Embed Size (px)
X-Ray Powder Diffraction and the identification and analysis of clay minerals-Preparatory and Interpretive Procedures1. Acetic acid treatment to remove carbonatesCarbonate rocks, or clastic rocks with significant carbonate contents, need to have the calcite or dolomite removed. However, treatment with strong acids to remove carbonate can attack the structure of clay minerals (e.g. trioctahedral minerals are often destroyed by such treatment), and even dilute acid can attack the silicate layers via interlayer regions and exposed edges. Generally, dilute acetic acid is preferred over hydrochloric acid because it less likely to affect clay crystallinity.
PROCEDURE FOR ACETIC ACID TREATMENT
Materials Required: glacial acetic acid distilled water glass graduated cylinder glass rod marking pencil 300-ml glass beakers glass pipette with rubber bulb siphon or centrifuge
Add 1 part acid to 4 parts distilled water in the graduated cylinder and mix throughly with the glass rod. Caution: acetic acid can cause burns. Wear safety goggles, plastic gloves, and an apron while working with this chemical.(Acetic acid 0.3 M or sodium acetate-acetic acid solution buffer at pH 5)
Label 300-ml beakers and add sample.
Add 50-75 ml of the acetic acid solution slowly to avoid foaming and overflow of beaker. A glass pipette may be used to transfer the acid solution. When effervescence subsides, add another 50-75 ml of acid. Stir and allow to stand overnight. Repeat until suspension no longer effervesces.Allow the suspension to settle and carefully siphon or pour off the supernatant liquid or wash sample by centrifuging. Dispose of acid waste properly.
2. Removal of organic matter with hydrogen peroxide[footnoteRef:1] [1: Commercial bleach is NaOCl (sodium hypochlorite) and seems quicker, cheaper, and safer (for your health) than the frequently recommended hydrogen peroxide; so the following procedure is recommended. Treat with 10 o 20 mL of NaOCl that has been adjusted to pH 9.5 with HCl just before treatment. Heat the mixture in a boiling-water bath abour 15 min. Centrifuge at 800 rpm for 5 min and decant and discard the supernatant. Repeat the procedure until organic material is sufficiently removed.]
Organic matter can produce broad X-ray diffraction peaks, increase the background, and inhibit dispersal of other minerals if present in significant amounts (a few percent). The organic matter can be removed chemically with strong oxidizing agents. Unfortunately, with H2O2 the danger is oxidizing octahedral iron and changing the layer charge. This is most likely with chlorite and vermiculite. The general rule (if there is one) is to go ahead with the peroxide treatment, but if you see some strange diffraction patterns that defy interpretation, suspect that iron oxidation has occurred. This is rarely the case under normal circumstances.
PROCEDURE FORTREATMENT WITH HYDROGEN PEROXIDE
Materials Required: Hydrogen peroxide (3%) glass graduated cylinder distilled water 300-ml glass beakers glass rod pencil squeeze bottle of distilled water lab tissues siphon
If the hydrogen peroxide is laboratory grade (30%), prepare a dilute solution of 3% using a graduated cylinder and distilled water.Caution: hydrogen peroxide is a strong oxidizer that can cause severe burns. Wear goggles, plastic gloves, and an apron while working with this chemical.
Label the beakers with a pencil or marker. Then, place a sample in each beaker and add about 50-100 ml of dilute hydrogen peroxide. Stir each beaker with the glass rod to suspend the sample. Rinse the glass rod between each sample and dry with a lab tissue. When bubbling stops or slows, add another 50-100 ml of dilute hydrogen peroxide and restir the suspension.
When the addition of hydrogen peroxide to the samples no longer causes bubbling, the organics have been removed. Allow the suspension to settle and carefully siphon or pour off the supernatant liquid, or wash the sample by centrifuging.
3. Randomly oriented powder mounts for x-ray powder diffractionBulk mineralogy of a sediment sample can be determined by X-ray diffraction with a randomly oriented powder mount. The random orientation insures that the incident X-rays have an equal chance of diffracting off any given crystal lattice face of the minerals in the sample. The use of a powder press to make randomly oriented powder mounts is undesirable because excessive force could cause preferred orientation of the crystallites. Although some orientation is inevitable (platy minerals tend toward some preferred orientation), the method described below is sufficient for most applications.Sample splits are commonly dried at 60 C prior to the preparation of randomly oriented powder mounts. The mounts are typically X-rayed between the angles of 2 and 70 degrees two theta using copper K radiation at a scanning rate of 2 degrees per minute.
PREPARATION OF RANDOMLY ORIENTED POWDER MOUNTS
Materials Required: plastic tape and pencil weighing paper (4"x4") mortar and pestle ASTM number 230 (.062 mm mesh) sieve stiff brush spatulas sample holders and clips glass microscope slide piece of glass slide cut to a size sufficient to cover the sample holder opening
Tape the glass slide over the opening of the sample holder. Leave tabs on each side for later removal of this cover, but fold the extra tape against itself so that it will not stick to other objects or the sample. Place the holder glass side down on a piece of weighing paper.
Grind the dried sample thoroughly so that it is easily brushed through the sieve. The particles should be much finer than .062 mm to avoid fractionation of the minerals. The sieve is used only to achieve even distribution and to ensure that the grinding is complete.
Place a second holder over the first as a mask. This enables the buildup of a thick enough layer of sample for later packing, while maintaining a clean metal surface on the final holder.
Place the sieve over the sample holder and brush the sample from the mortar. (Note: the sample may become contaminated from the sieve and utensils. These contaminants will not affect the x-ray diffraction analysis, but do not plan to reuse this cut of the sample for sensitive chemical analyses.)
Use the spatula to loosen any sample that has stuck to the mortar and brush the material into the sieve.
Brush the sample through the sieve into the cavity of the sample holder. The purpose of the brushing is to obtain an even distribution and to minimize preferred orientation of the particles.
Remove the sieve and mask.
Place the sample holder on a clean piece of weighing paper, tap the powder remaining on the mask onto the first weighing paper, and replace the mask over the sample holder.
Pour the excess powder onto first weighing paper into the sample holder. Distribute the powder evenly.
Use a glass slide to pack the sample into the cavity firmly enough so that it will not fall out, deform, or slide, but not so firmly that preferred orientation will be produced on the opposite surface (which will later become the top surface). The glass slide can also be used to scrape any sample that has flattened onto the holder surface during packing back over the holder opening.
Additional sample can be used as filler if necessary to create a firm pack. This part of the sample need not be as finely ground, as it will become the bottom surface and will not be exposed to the X-ray beam.
Pack as above and then attach a clip to the back of the holder. Alternately, if a generic holder is being used, another cut glass slide can be attached with tape to cover the holder's opening.
Turn the sample holder over and lift the tab of tape. The glass cover is carefully lifted with a slight twisting motion to break and surface adhesion. This will be the surface exposed to the X-rays. It should be smooth, uniform, and flush with the metal surface of the holder. If not remake the mount.
Label the sample holder with the pencil.
4. Smear slide sample mounts for x-ray powder diffractionFor identifying the constituents in a bulk sample and roughly estimating the quantities, the smear technique is a good compromise between time and skill required and the quality of the results. Done properly, phases should be represented in their true proportions, i.e., without segregation. Although not useful for semi-quantitative analysis, this method is useful for rapidly determining bulk mineralogy, especially if the operator knows which mineral phases are likely present.PREPARATION OF SMEAR-SLIDE MOUNTS
Materials Required: weighing paper (4"x4") mortar and pestle spatula glass rod marker pen glass slide cut to fit the diffractometers'ssample holder acetone in a squeeze bottle lab tissues diamond or carbide scribe to cut slides
Grind the dried sample thoroughly with the mortar and pestle. The particles should be much finer than .062 mm to avoid fractionation of the minerals. The finer the powder the greater the opportunity for obtaining an adequate number of particles with random orientation and the less likely that surface roughness will reduce low-angle intensities.
Use the spatula to loosen any sample that has stuck to the mortar and to homogenize the powder.
Place a small amount of sample in the center of the slide and add an amount of acetone sufficient to wet the sample (2-3 drops). Distilled water may be used, but the sample dries quicker with acetone.
Spread the sample into a thin layer with the glass rod. Gently blow on the slide to rapidly evaporate the acetone. Use the spatula or a finger to remove any excess sample sticking to the edges of the slide. Use a lab tissue to remove any sample stuck to the back of the slide.
Label the slide with a marke